Industrial Crops and Products 62 (2014) 179–187
Contents lists available at ScienceDirect
Industrial Crops and Products journal homepage: www.elsevier.com/locate/indcrop
Wood ﬂour modiﬁed by hierarchical Ag/ZnO as potential ﬁller for wood–plastic composites with enhanced surface antibacterial performance Pavel Bazant, Lukas Munster, Michal Machovsky, Jakub Sedlak, Miroslav Pastorek, Zuzana Kozakova, Ivo Kuritka ∗ Centre of Polymer Systems, University Institute, Tomas Bata University in Zlin, Nad Ovcirnou 3685, 760 01 Zlin, Czech Republic
a r t i c l e
i n f o
Article history: Received 1 May 2014 Received in revised form 11 August 2014 Accepted 14 August 2014 Keywords: Wood ﬂour Modiﬁcation Nanosilver Zinc oxide Wood–plastic composite Antibacterial
a b s t r a c t In order to extend application potential of wood–plastic composites (WPC) in interiors with respect to hygienic requirements, wood ﬂour (WF) was modiﬁed by nanosilver, nanostructured ZnO and hybrid nanostructured Ag/ZnO surface decorations. A microwave assisted solvothermal synthesis method was employed starting from soluble precursors. Composition of source chemicals and synthesis protocol were intentionally varied to prepare different materials and elucidate the reaction mechanism. Obtained modiﬁed wood ﬂour were compounded into a model PVC matrix to assess their antibacterial performance. The surface antibacterial activity was tested according to ISO 22196: 2007 (E) standard. Single silver or ZnO modiﬁed WF have signiﬁcantly lower efﬁciency than hybrid Ag/ZnO decorating the surface of WF particles. A simple variation of the synthesis method by additional ammonia precipitation step increased largely the performance of the material and excellent efﬁciency comparable with contemporary medical grade materials was achieved, suggesting the great application potential of investigated systems in WPCbased materials. © 2014 Elsevier B.V. All rights reserved.
1. Introduction Wood ﬂour (WF) originally represented a waste material which was actually needed to be removed from sawmills in the past. Many waste management strategies have been introduced over last century, such as bedding, composting, combustion, gas generation, use as feedstock for chemical industry etc. Among them the use of WF as raw material for making new solids is the most favourable due to its straightforwardness in application and low energetic costs. These advantages make WF one of the most abundant yet valuable materials. Due to the need of replacing pressure-treated solid lumber, wood plastic composites (WPC) have been developed successfully in the last decades, and have been arousing great interest as important engineering materials (Ashori, 2008; Okamoto, 2003). They have become commonly used in many exterior and interior applications, such as in buildings, decking, automotive, highway
∗ Corresponding author. Tel.: +420 576 038 049; fax: +420 576031444. E-mail addresses: [email protected]
(P. Bazant), [email protected]
(L. Munster), [email protected]
(M. Machovsky), [email protected]
(J. Sedlak), [email protected]
(M. Pastorek), [email protected]
(Z. Kozakova), [email protected]
(I. Kuritka). http://dx.doi.org/10.1016/j.indcrop.2014.08.028 0926-6690/© 2014 Elsevier B.V. All rights reserved.
construction, fencing and many other (Fowler et al., 2006; Karas and Muszynski, 2011; Lin and Renneckar, 2011). The industrial applications frequently join the recyclable or recycled thermoplastic polymers as matrices in composite materials with the WF ﬁller to save costs as the WF is a by-product of lumber processing. (Najaﬁ, 2013) Completely renewable materials are tested as well, e.g. WF compounded into polylactide matrix (Hrabalova et al., 2010). The emphasis in development of these products is usually put on the sustainability issue. However, nowadays, the attention has been targeted to improvement of the composite performance, instead of just simple replacement of expensive recent material by its cheaper substitute with barely sufﬁcient properties. Silylation, acetylation and melamine–formaldehyde surface modiﬁcation of WF are used for improving the interfacial adhesion of the polar wood ﬁller surface with hydrophobic polymer matrix (Muller et al., 2013). Besides chemical treatment, the WF is supplemented by addition of many co-ﬁllers enhancing the performance of the composite in desired functionality. Carbon and glass ﬁbres, clay minerals are often employed to name a few. Nanotechnology came to assist recently with the application of nanoﬁllers (Li et al., 2013; Turku and Karki, 2014a, 2014b).
P. Bazant et al. / Industrial Crops and Products 62 (2014) 179–187
The highly hydrophilic characters of lignocellulosic materials make them susceptible towards various biotic degradation factors and prone to microbial decay. With the exception of controllable biodegradable materials, any outdoor application requires some resistance of the composite material to the attack of water and humidity, weather, soil and living organisms. Much of the research on WPCs has been focused on formulation development and processing while high biological durability of the material was assumed. However, the gap between assumption and knowledge in biodeterioration of WPC still needs to be reduced and efﬁcient strategies need to be developed to improve the performance of these relatively new materials and to enable use of WPC for many demanding applications (Schirp et al., 2008). In order to overcome the inclination of wood ﬂour based WPCs to decay caused by biotic factors, various approaches are used for imparting the antimicrobial resistivity to the composite material. Careful selection of WF sources, their composition and manufacturing conditions of WP is necessary (Benthien et al., 2012; Schilling and Norcutt, 2010; Xu et al., 2013). With respect to the bio-deterioration of the materials, main attention is devoted to antifungal modiﬁcations (Naumann et al., 2012; Simonsen et al., 2004) and to additional improvement of termite resistance for application in many parts of the world (Kartal et al., 2013; Lopez-Naranjo et al., 2013; Schauwecker et al., 2006). Allyl alcohol and its copolymers (Solpan and Guven, 1999), styrene and glycidylmethacrylate (Devi and Maji, 2008) can be used for WF pretreatment to enhance the WP performance. Materials based on copolymers of lignin and synthetic monomers have been introduced already, although they require substantial chemical alteration and processing of the original WF (Huttermann et al., 2001; Lin and Renneckar, 2011). Among inorganic chemical treatment methods, boric acid and borates were successfully applied (Simonsen et al., 2004), especially the zinc borate (Tascioglu et al., 2013) combining the effect of boric compounds with antimicrobial action of zinc(+II) form. Generally, a lot of effort is spent to suppress the deterioration of WP by living organisms in outdoor exposure. On the other hand, in-door applications of WP have different purposes and conditions of use. Many of interior WP products are expected to meet hygienic criteria to assure the protection of the population and to help keep the personal well-being of individuals. Although this function is related to the resistance against biodeterioration, other factors become crucial for the material performance and new strategies for best achievements have to be formulated. The in-door application may put to some extent less strict requirements on the resistivity of the material to biodegradation, but the hygienic standards require reducing of the microbial adherence and colonisation of the WPC’s surface. Various organic and inorganic antibacterial additives impart the biostatic or biocidal property to the inactive polymer matrix and advanced plastic materials are prepared with reasonable surface antibacterial performance. Among them, composite materials combining excellent properties of inorganic nanoparticles and polymers have been developed recently. They were often studied with the aim to be used in highly demanding applications, such as biomedical materials etc. A lot of good examples can be found and one can learn much from these branches, especially in hygienic materials or textiles (Dastjerdi and Montazer, 2010; Guo et al., 2013; Marambio-Jones and Hoek, 2010). Currently available inorganic antibacterial polymer systems most often rely on silver nanoparticles (Dwivedi et al., 2013; Guzman et al., 2012; Jayakumar et al., 2012; Llorens et al., 2012). Zinc and other metallic oxide nanoparticles are utilised in formulations too (Droval et al., 2014; Farouk et al., 2014; Gowri et al., 2010; Llorens et al., 2012; Seil and Webster, 2011; Schwartz et al., 2012). Both materials can be used in hybrid Ag/ZnO system which shows synergy in effect and thus enhanced performance (Sadeghi, 2014; Zhang et al., 2014). Easily processable hierarchical Ag/ZnO ﬁller has been developed
and proved as suitable material for even highly demanding applications in medical materials (Bazant et al., 2014). We extended this approach and modiﬁed the surface of WF particles by the Ag/ZnO nanostructured decorations which impart excellent surface antimicrobial activity towards human-pathogenic bacteria. To the best of our knowledge, no published reports are available regarding the effect of Ag/ZnO modiﬁed WF on the antibacterial properties of WPC. In this study, WF was not used as reinforcing ﬁller but as a carrier for hybrid Ag/ZnO nanostructured ﬁller. First, fast microwave solvothermal synthesis method was used to modify neat WF (nWF). Soluble silver nitrate and zinc acetate as metal ion sources and hexamethylenetetramine served as precipitating and reducing agent. Two synthetic routes employing microwave (MW) heating were examined. After structural and morphological characterization, modiﬁed WF (m-WF) was compounded with polymer matrix and tested according to ISO 22196: 2007 (E) (2007) to demonstrate the antibacterial performance of the ﬁller at 5 %wt loading level. The well-known plasticized PVC was used as a model matrix material–a kind of standard. The choice of the PVC matrix was considered in view of a report on PVC matrix based WP also (Muller et al., 2013) however the plasticized compound was preferred due to its easiness of processing.
2. Experimental 2.1. Materials Zinc acetate dihydrate Zn(CH3 COO)2 ·2H2 O, Silver nitrate AgNO3 , hexamethylenetetramine (CH2 )6 N4 (HMT) and aqueous ammonia (28–30 %wt) were all purchased from PENTA (Czech Republic) and used as received without further puriﬁcation. Soft wood ﬂour BK 40-90 was supplied by J. Rettenmaier & Söhne GmbH + Co.KG (Germany). The producer declared following properties of WF: Particle size main 300–500 m; pH 4.5-6.5; bulk density 170–230 g/L. Distilled water was used throughout whole experiments. Plasticized PVC RB3 was used for composite preparation. The resin was supplied by Modenplast Medical S.r.l. (Italy).
2.2. Modiﬁcation of wood ﬂour by Ag/ZnO In all experiments, 1 g of WF was dispersed in 30 mL of distilled water and stirred by a magnetic stirrer for 30 min prior to process of modiﬁcation. Meanwhile, solutions of Zinc acetate dihydrate and Silver nitrate were prepared separately by dissolving in 70 mL of distilled water to be used as source of Zn2+ and Ag+ . If only one source salt was used, 70 mL of water was used for preparation too in order to keep the target initial volume 100 mL of water in the reaction mixture of WF and salts constant in all experiments. Obtained solution and WF dispersion (i.e. 70 + 30 mL) were transferred into 250 mL reaction bottle suitable for MW heating. The precipitation reaction was performed under reﬂux in the MW open vessel system MWG1K-10 (RADAN, Czech Republic; 1.5 kW, 2.45 GHz) operated in continuous mode (zero idle time) with external cooler. The reaction mixture was always preboiled in MW oven for 10 min. After that, 50 mL of water with dissolved load of HMT was added and the MW heating continued for 10 min. In case of samples denoted with AA in the sample code, additional amount of aqueous ammonia was added and the MW heating was prolonged for another 10 min. For detailed information about reaction mixture composition, see Table 1. The value of pH was measured by a pH Meter Lab 870 (Shott Instrument, AG Germany) equipped with a glass electrode. The product was collected by suction microﬁltration and left to dry in a laboratory oven up to the constant weight. Each synthesis
P. Bazant et al. / Industrial Crops and Products 62 (2014) 179–187
Table 1 Overview of samples, sample codes, amounts of used chemicals and average synthesis yields. Sample code
Precursor of Zn2+ (g)
Precursor of Ag+ (g)
WF-Ag WF-ZnO WF-Ag/ZnO WF-Ag-AA WF-ZnO-AA WF-Ag/ZnO-AA
1.000 1.000 1.000 1.000 1.000 1.000
– 10.800 10.800 – 10.800 10.800
0.701 – 0.701 0.701 – 0.701
6.928 6.928 6.928 6.928 6.928 6.928
NH3 aq.(mL) – – – 14.2 14.2 14.2
Yield(g) 1.38 1.66 1.89 1.38 4.05 4.56
was repeated several times to obtain sufﬁcient amounts ﬁller for all experiments.
composites fractured surfaces in order to evaluate the degree of homogeneity and to gain insight into composites internal structure.
2.3. Preparation of composites
2.5. Antibacterial activity testing
The PVC composites containing modiﬁed WF and one composite containing n-WF were prepared by melt mixing of PVC pellets with appropriate amount of prepared ﬁller in a Brabender measuring mixer W50 EHT PL at the temperature 175 ◦ C. The ﬁller concentration was 5 wt% in all samples. The rotor speed was kept at 20 rpm for ﬁrst 2 min followed by increase to 50 rpm for another 4 min. After completion of this time, constant torque was stabilised that signalised achievement of homogeneous mixing of ﬁller into matrix. Than, 1 mm thick sheets were produced by hot press procedure involving preheating at 175 ◦ C for 2 min followed by compressing for 4 min and subsequent cooling under pressure. Neat PVC reference sample without any WF was prepared in the same way. Obtained sheets were used as testing samples for evaluation of antibacterial activity. The encoding of prepared composites is obvious. It contains an acronym for used ﬁller in accordance with ﬁller coding indicated in Table 1 a slash and code for the matrix PVC. The composite with n-WF is simply denoted as WF/PVC; neat PVC has no special code.
The antibacterial activity of prepared composites was assessed against Escherichia coli ATCC 8739 and Staphylococcus aureus ATCC 6538P according ISO 22196: 2007 (E). For the sake of clariﬁcation, a brief description of this standard assay for evaluation of antibacterial activity on plastic surfaces is given. First, a test inoculum was prepared by transferring one loop of the pre-incubated bacteria into a small amount 1/500 diluted nutrient broth. The test specimens (three specimens made from each composite including WF/PVC and three untreated made form neat PVC) with dimensions 50 mm × 50 mm × 1 mm were placed in Petri dishes and inoculated by 0.4 mL of the test inoculum. Inoculated specimens surface was covered with thin piece of polypropylene ﬁlm (40 mm × 40 mm) and pressed down gently so that test inoculum spread to the edges. After incubation for 24 h at 35 ◦ C under humid condition (95%), test inoculum remaining on covers ﬁlm and test specimen was completely recovered by 10 mL of SCDLP broth (prepared by adding 1 g of lecithin and 7 g of polysorbate per litter of Tryptone Soya Broth). Recovered SCDLP broth was 10-fold serial diluted in phosphatebuffered physiological saline and 1 mL of each dilution was placed together with 1 mL of undiluted recovered SCDLP into separate Petri dishes. 15 mL of plate count agar was poured into each Petri dish, swing gently to disperse bacteria and incubated for 48 h at 35 ◦ C under humid condition (95%). After incubation, the number of colonies was counted in the Petri dishes containing from 30–300 colonies.
2.4. Characterization The crystalline phase structure was identiﬁed by powder X-ray diffraction (XRD). The XRD patterns of prepared m-WF ﬁllers were recorded by the multi-purpose X-ray diffractometer X´ıPert PRO MPD (PANalytical, The Netherlands) with a Cu-K␣ X-ray source ˚ in the diffraction angle range 5–85◦ 2. The phase ( = 1.5418 A) composition was evaluated by the use of PANalytical X’Pert HighScore software using the ratio between the integrated normalised intensities of the peak of interest and that of a known standard. The morphology and structure of ﬁllers were observed by scanning electron microscope Vega II/LMU (Tescan, Czech Republic). Scanning electron microscopy examination was also performed onto
3. Results and discussion 3.1. Modiﬁcation of WF The size and shape of particles of n-WF can be seen in Fig. 1A. The morphology of n-WF used throughout these experiments
Fig. 1. SEM images of n-WF at lower (A) and higher (B) magniﬁcation.
P. Bazant et al. / Industrial Crops and Products 62 (2014) 179–187
Fig. 2. SEM microphotograph of samples, where (A) WF-Ag; (B) WF-ZnO; (C) WF-Ag/ZnO; (D) WF-Ag-AA; (E) WF-ZnO-AA; (F) WF-Ag/ZnO-AA.
is exempliﬁed on a more detailed SEM image of a particle in Fig. 1B. Tracheides, typical structural features for softwood can be observed. The morphology retained from the original wood structure enlarges the speciﬁc surface and is responsible for the evidently rugged topography of the particle surface. The tracheides enhance the wettability and imbibition capacity of the ﬁller if it comes in contact with water which is favourable during our modiﬁcation procedure. In order to investigate the individual contribution of silver, ZnO or Ag/ZnO hybrid and the inﬂuence of modiﬁcation procedure too, a set of six samples was prepared as indicated in Table 1. Morphology of obtained products is shown in the set of SEM images in Fig. 2. Recorded X-Ray diffractograms are shown in Fig. 3 and the
Fig. 3. XRD patterns of m-WF decorated by Ag, ZnO and Ag/ZnO particles obtained by the two synthetic methods; symbols represent diffraction peaks of metal silver (full circles, 䊉), ZnO (crosses, +) and wood ﬂour cellulose (hollow circles, ).
Table 2 Summary of XRD analysis: Weight ratio of inorganic phases in m-WF and size of nanocrystallites of silver and ZnO obtained by Scherrer formula from line broadening. Sample code
WF-Ag WF-ZnO WF-Ag/ZnO WF-Ag-AA WF-ZnO-AA WF-Ag/ZnO-AA
Composition of inorganic crystalline phase in m-WF
Diameter of nanocrystalline diffracting volume
100 – 24 100 – 10
– 100 76 – 100 90
15 – 19 16 – 17
– 33 47 – 44 54
results phase composition analysis and peak broadening analysis are summarised in Table 2. In all cases, the surface of m-WF particles was decorated by precipitated particles. The distribution of particles was always quite homogeneous and no large uncovered (bare) surface areas were observed. On the other hand, the contiguity of the surface coverage by the particles was not complete and individual particles separated from other can be seen in some cases, while agglomeration dominates the distribution in other cases. In general, different coverage modes and hierarchies were observed in dependence on the reaction mixture composition and NH3 aq addition. Silver nanoparticles precipitated by HMT from silver nitrate solution only (sample WF-Ag in Fig. 2A) were found to be attached to the whole surface of the WF particle including cavities and tracheides. However, the particles tend to agglomerate and preferentially attach to the edges of longitudinally cut tracheides. Agglomeration into cake-like structures was observed to a smaller extent, but even in such case the particles were attached to the m-WF surface. The development of Ag crystalline structure can be followed in the diffractogram in Fig. 3. Simple cubic phase of Ag0 corresponding to JCDD PDF-2 entry 01-087-0720 was identiﬁed. The peaks are evidently broad and were further analysed with the use of Scherrer formula. The average size of metallic silver nanocrystalline domains was about 15 nm (Table 2). Surface of WF modiﬁed by ZnO precipitated by HMT is presented in Fig. 2B. Typical drum-like hexagonal frustums and apically joined
P. Bazant et al. / Industrial Crops and Products 62 (2014) 179–187
bifrustums can be seen on the surface of WF-ZnO. They are about 1–2 m in size. They do not show any preferential crystal wall joining to the WF surface and cover it with homogeneous distribution. Isolated objects as well as not numerous clusters may be found. In many cases it can be seen that the particles are hollow, resembling thus nuts, hexagonal boxes, sandglass or shape of the cezve but without the long handle. The particles are sometimes capped, so the inner cavity (hole) cannot be seen always. In some cases, a porous and mostly incomplete soft ﬁlling can be observed is most likely an intermediate in growth of the particles which is consumed during the growth of the lateral surface walls (facets) of the prism on the expense of the intern of the particle and cavity formation. Similar cup-like structures were already observed by other authors (Zhao et al., 2009). Wurtzite structure was conﬁrmed for prepared ZnO crystalline phase by XRD (see Fig. 3) by the perfect agreement of diffracting lines positions with JCDD PDF-2 entry 01-079-0207. The peak broadening in the powder X-Ray diffractogram can be observed in Fig. 3 too. The average crystallite size was estimated about 33 nm (Table 2) which conﬁrmed the complexity of ZnO decoration morphology although it cannot be directly attributed to the wall thickness of the hollow frustums because contributions of all diffracting areas are smeared together by averaging. Combination of Zn2+ and Ag+ source solutions resulted in decoration of the WF-Ag/ZnO surface by particles of both kinds. It seems that ZnO microparticles are slightly smaller in comparison with WF-ZnO (compare Fig. 2B and C) however the nanocrystallite size is somewhat bigger according to the peak broadening analysis (Table 2). This effect is more pronounced for ZnO than for Ag nanodomains. It can be explained by the role of silver ions as monovalent Ag (+I) impurity in ZnO crystals which enhances the diffusion of vacancies during ZnO crystal phase growth process (Chauhan et al., 2012). Silver nanoparticles form smaller and not numerous agglomerates. The signiﬁcant agglomeration of silver nanoparticles along edges on WF surface was not observed. The composition of crystalline phases ZnO:Ag was approximately 3:1 by weight. The morphology of the second triad of samples which were prepared by additional aqueous ammonia precipitation is shown in lower row of images in Fig. 2, i.e. 2D, 2E and 2F. The NH3 aq addition did not practically inﬂuence the material WF-Ag-AA in comparison with WF-Ag. The size of nanocrystalline diffracting domains remained nearly unchanged (Table 2). Only the tendency to agglomeration along edges was less manifested. Pronounced changes were observed in the next composition. The surface of WF-ZnO-AA is covered by slightly more ZnO microparticles of approximately the same size as in WF-ZnO, but this is all similarity which can be found between these two samples and there are many differences observable on closer look. The size of diffracting nanodomains is bigger than it was observed for material without NH3 aq addition (44 nm in comparison with 33 nm, Table 2). The shape of ZnO microparticles is rather more like a twinned hexagonal prism than cezva-like as in WF-ZnO. Moreover, the rods are only rarely hollow or have much smaller and less developed central cavity of irregular shape. The prisms seem to have the internal space ﬁlled by porous ﬁlling. A second generation of ZnO particles growth of which is induced by NH3 aq addition is represented by small rods sparsely distributed on the WF surface between the prisms. These tool rods are of submicrometric dimensions (length about 500 nm and diameter less than 100 nm) and they grow on the WF substrate isolated from each other. However in this case they form a brush like structure as multiple rods grow side by side perpendicular only from the basal face of prisms which are not twinned. This hierarchical morphology strongly resembles observations of (Cho et al., 2008) and the small nanorods can be denoted as cake candles too. The addition of NH3 aq to the reaction mixture caused extreme changes in the WF-Ag/ZnO-AA product morphology in comparison to WF-Ag/ZnO. The main difference is that the single rods
(nanowires) densely cover the surface of m-WF particles resembling thus a forest between the twinned prism ZnO microparticles. The density of the nanorods population can be explained by the nucleation effect of silver nanoparticles (Fan et al., 2009). The morphology of ZnO prisms remained the same including the secondary growing rods on their bases, they only look slightly bigger. A third hierarchical level of nanoparticles may by observed as very ﬁne cotton wool. The average size of ZnO nanocrystalline domains is about 54 nm which is the biggest among prepared samples. However, it can be hardly said what all contributes to the line broadening, as there are evidently three size hierarchies of ZnO nanostructures. According to the size analysis with the use of Scherrer equation, the silver nanoparticles were not altered signiﬁcantly and their size remained about 17 nm. According to the microscopic observation, we consider them to be buried beneath ZnO nanorods most likely as nucleating sites.
3.2. Notes on chemistry of the WF modiﬁcation There are two basic factors inﬂuencing the chemistry of the modiﬁcation process. First, the properties of n-WF surface are crucial with respect to the attachment of synthesised particles to the substrate which can be inﬂuenced by the WF selection. Secondly, the composition of the reaction mixture and wet process conditions of WF modiﬁcation can be intentionally chosen in order to inﬂuence the resulting surface decoration and its properties. The solvothermal synthesis combined together with MW heating offer large variability in particle design which can be accomplished within very short reaction time (Bazant et al., 2014). Three main components can be expected to form the surface of n-WF: cellulose, hemicellulose and lignin. The ﬁrst two of these macromolecular compounds are highly polar and contain abundant hydroxyl or carbonyl groups. Lignin is more hydrophobic than the two polycarbohydrates creating cell walls because lignin comprises non-polar components besides polar functional groups. The surface of the n-WF particles is large due to the naturally porous morphology of wood. Milling can contribute by creation of edges and splintery fractures too. Therefore, we soaked the n-WF in distilled water for 30 min prior any other manipulation to saturate the surface and especially all cavities and pores of n-WF particles by water in order to enhance diffusion of soluble precursors to the whole surface of particles. This initial operation was followed by mixing of the n-WF dispersion in water with solution of precursors. Obtained reaction mixture was further heated by MW for ten minutes to agitate the adsorption of Ag+ , Zn2+ or both species to the surface. No precipitation of white zinc containing compounds was observed at this stage. On the other hand, darkening of WF was observed for silver source solutions. Natural wood can contain reducing groups and can contribute to silver ion reduction even at this stage. Moreover, various silver to oxygen containing group bonding conﬁgurations for adsorbed Ag+ may form. These adsorbed or coordinated sites can play the role of nucleation sites for silver nanoparticle formation in the next reaction step, when HMT is added. The HMT decomposes slowly at high temperature in aqueous solution according to following equation: (CH2 )6 N4 + 6H2 O → 4NH3 + 6HCHO
This reaction is responsible for gradual increase of pH during reaction as the NO3 − anion does not undergo hydrolysis and the solution of the source salt has no buffer capacity. The increase of ammonia concentration and pH causes formation of complex Ag(+I) cations: Ag+ + 2NH3 → [Ag(NH3 )2 ]+
P. Bazant et al. / Industrial Crops and Products 62 (2014) 179–187
which undergoes easily to the reduction caused by formaldehyde released from HMT too: HCHO + 2[Ag(NH3 )2 ]+ + H2 O → HCOO− + 2Ag0 +3NH4 + + NH3 (3) Formation of silver nanoparticles out of the surface of WF particles was not observed in microscopic observations and all particles were found to be attached to the m-WF surface or to agglomerates sessile on the m-WF surface. It can be suggested that pre-adsorbed Ag+ on the WF surface fulﬁls the role of nucleation sites. Similarly, Zinc(+II) species can be adsorbed and coordinated on the WF surface and may play the role of initial nucleation seeds. However, observed synthesised particles (the twinned bifrustums) are quite big, do not form a dense population on the WF surface and do not show any preferable crystal facet which would serve to anchor the microparticle to the surface. The Zn(+II) source salt is an acetate containing thus an anion which hydrolyses and therefore, the pH remain nearly the same during the second reaction step as at the beginning of the reaction, i.e. about 6.1-6.4 irrespectively to the degree of HMT decomposition according to the Eq. (1). According to the reference (Richardson and Lange, 2009), the speciation of Zn(+II) compounds strongly depends on both pH and temperature in presence of ammonia in the solution. The cation ZnOH+ is the prevailing Zn(+II) species in our pH range at the temperatures nearly to the boiling point. At the laboratory temperature Zn2+ would prevail. Although the HMT is the source of ammonia, [Zn(NH3 )4 ]2+ cations would scarcely formed under weak acidic condition. Bound water molecules are neglected in used notation. The thermodynamic analysis supports strongly the model of reaction mechanism involving primary precipitation of layered zinc hydroxy acetates (Biswick et al., 2009): 5Zn2+ + 2CH3 COO− + 8OH− + (n)H2 O → [Zn5 (OH)8 (H2 O)2 ](CH3 COO)2 ·(n − 2)H2 O
Where n can be 2, 3 or 4. This mechanism is in accord with our visual observation of very fast precipitation of white product immediately with the addition of HMT. The decomposition of HMT is the source of hydroxide ions and the role of HMT at used concentration range is replenishment of hydroxide ions consumed into growing precipitate and production of NH4 + involved in the complicated interplay of chemical equilibria. Ammonium acetate solution provides further buffering capacity. The hydrolysis of acetate ion as the source of hydroxides can be sufﬁcient for precipitation only at very high temperatures and pressures as it was shown in single source water system resulting in ZnO cup-like microparticles (Zhao et al., 2009). In the synthesis of ZnO decorated ﬁllers, formaldehyde can play only secondary role if any. Formation of this layered compound is followed by their transformation into ZnO wurtzite phase at elevated temperature giving rise to the typical bifrustum like microparticles. [Zn5 (OH)8 (H2 O)2 ](CH3 COO)2 ·(n − 2)H2 O → 5ZnO + (n + 1)H2 O + 2H3 O+ + 2CH3 COO-
The transformation into ZnO phase can be fully completed within ten minutes. (Golic et al., 2011) Released acetic acid neutralises further with decomposition product of HMT. It must be noted, that the Eq. (5) is only a summary equation and does not represent the mechanism of solid phase transformation. Similar equation was proposed for synthesis of ZnO via zinc hydroxy acetates (Golic et al., 2011) however we rebalanced and corrected the Eq. (4) in comparison with that study.
A combined mechanism is expected in the case of WF-Ag/ZnO preparation. The HMT serves as the source of NH4 + and HCHO and the reactions according to Eqs. (2)–(4) can run parallel. Indeed, only slight dependency was observed between the product morphology and other structural properties of ZnO besides Ag nanoparticles. It can be said that the reactions are competitive to some extent as they share one source compound, the HMT. The mass of inorganic decoration on WF-Ag/ZnO (0.89 g) is slightly less than a sum of Ag (0.38 g) and ZnO (0.66 g) contributions in WF-Ag and WF-ZnO. (See Table 1.) The addition of ammonia in the third reaction step did not practically inﬂuence formation of silver nanoparticles at sample WF-Ag-AA, but microparticles of ZnO were inﬂuenced signiﬁcantly in case WF-ZnO-AA. Therefore, we consider the formation of Ag nanoparticles is ﬁnished at the end of the second step. Theoretically 0.445 g of silver metal could be obtained from used load of silver nitrate. Observed yield is about 0.38 g, which corresponds to the 85% of theoretical value. The addition of NH3 aq in the third reaction step increases suddenly the concentration of ammonia by addition of cca 0.2 mol of NH3 which corresponds to the increase of ammonia concentration by 1.2 mol/L. The addition most likely overbalances the buffer capacity of the reaction mixture and pH increases, theoretically up to the value about 11.5. However, the addition occurs at elevated temperature under reﬂux, so the pH will not increase that much, as the pH of water solution generally decreases with increasing temperature due to increased self-dissociation of water. Increased temperature supports the precipitation of ZnO because the solubility of ZnO decreases in ammonia solutions with elevating temperature. The solubility range of [Zn (NH3 )4 ]2+ which is at room temperature up to the pH 11.5 shrinks with increasing temperature as well and shifts to lower values as the solution is heated and we expect it to be in range 11–11.5 (Richardson and Lange, 2009). According to the obtained yield, most of the zinc source compounds remain in the solution at the end of the second reaction step. The initial load of zinc acetate contains theoretically 4 g of ZnO and only 0.66 g was observed as the increase in mass for the sample WF-ZnO which corresponds to the 17% of the theoretical yield. Therefore, we suggest that at the second reaction step, dissolved Zinc(+II) species remain mostly in the solution. Cations Zn2+ , ZnOH+ and [Zn(NH3 )4 ]2+ may coexist at various concentrations at given pH and temperature. The sudden increase of ammonia concentration caused by NH3 aq addition converts them into [Zn(NH3 )4 ]2+ according to Eqs. (6) and (7) at the beginning of the third step. However, as the pH is about 11–11.5 and the temperature is at the boiling point, the speciation shifts and a transition from positively charged [Zn(NH3 )4 ]2+ to negatively charged species as Zn(OH)3 − and Zn(OH)4 2− occurs. (Richardson and Lange, 2009) Then, it is followed by fast precipitation of ZnO according to Eqs. (9) and (10) rather than according the Eq. (8) which is more likely the reaction pathway for lower (room) temperatures although its occurrence cannot be fully excluded because the reaction system was always left to cool down prior ﬁltering. However, immediately after ammonia addition we always observed vivid stimulation of the reactions in the system and increased precipitation. Therefore, formation of zinc hydroxide complex anions as the intermediate reaction step is a reasonable explanation for the reaction mechanism. Zn2+ + 4NH3 → [Zn(NH3 )4 ]2+
ZnOH+ + 4NH3 → [Zn(NH3 )4 ]2+ + OH−
[Zn(NH3 )4 ]2+ + 4H2 O → ZnO + 2OH− + 4NH4 + + H2 O
Zn(OH)3 → ZnO + H2 O + OH
Zn(OH)4 2− → ZnO + H2 O + 2OH−
P. Bazant et al. / Industrial Crops and Products 62 (2014) 179–187
Fig. 4. SEM microphotograph of WF/PVC composites where (A) WF-Ag/PVC; (B) WF-ZnO/PVC; (C) WF-Ag/ZnO/PVC; (D) WF-Ag-AA/PVC; (E) WF-ZnO-AA/PVC; (F) WF-Ag/ZnOAA/PVC.
These consecutive and parallel reactions may contribute to the faster maturation and secondary growth of ZnO twinned prisms together by suppression of the formation of the internal cavities. In next, higher concentration of ammonia and thus higher pH induced growth of the second generation ZnO rod-like nanoparticles sparsely distributed on the WF surface. Formation of these objects was described earlier for ZnO precipitation of so called nanowires (Cho et al., 2008). Similarly, the cake candle-like structures were observed (see Section 3). The mass of inorganic decoration on WF-ZnO-AA signiﬁcantly increased (3.05 g) as can be seen Table 1. Such value corresponds to 75% of the theoretical yield. The effect of addition of NH3 aq is most pronounced at sample WF-Ag/ZnO-AA. It was most likely the dense surface coverage by Ag nanoparticles what caused efﬁcient nucleation and growth of nanowires. It was already observed that nanosilver is a very good nucleating seed for ZnO (Fan et al., 2009). The mass increase of the sample WF-Ag/ZnO-AA in comparison with the initial amount of WF is 3.56 which is nearly the sum of Ag and ZnO yields from WF-Ag-AA and WF-ZnO-AA. To complete the discussion, it must be mentioned that one of the most generally known reactions of NH3 aq with lignin is the cleavage of C O C bonds in lignin as well as ether and ester bonds in the lignin-carbohydrate complex. However we did not observe signiﬁcant erosion or deterioration of the m-WF particles. Possible partial deligniﬁcation and release of its hydrolysis products might serve as a source of surface stabilizing and capping agents however we have no indications supporting such hypothesis yet and further research work is required as this question remains opened. Similarly, it is well known, that Zn(OH)4 2− may swell cellulose and this issue requires further studies too with respect to our system. 3.3. Characterization of WF/PVC composites The morphology of prepared WF/PVC composites was analysed with the SEM microscopy on cross sections shown in the Fig. 4. The poor surface adhesion of PVC matrix to the WF ﬁller was not improved by decoration by Ag, ZnO or Ag/ZnO micro- and nanoparticles. It is evident that the morphology of ﬁllers and their components was not altered by the process of compounding and
that the most of Ag and ZnO material remained attached to the surface of WF particles. On the other hand, some of the Ag and ZnO particles were peeled off from the m-WF surface and dispersed into the entire volume PVC matrix during compounding. Such disagglomeration can be considered as a positive effect as it can only improve the expected antibacterial property of the material. The relatively low used ﬁller concentration should not inﬂuence the mechanical properties of plasticised PVC dramatically. On the other hand, the antibacterial activity must be signiﬁcantly manifested if the ﬁller can truly impart this desired property to prepared compounds even at 5 %wt loading. Therefore, we focused only on testing of the surface antibacterial activity against the two bacterial strains representing Gram positive and Gram negative bacteria. E. coli and S. aureus were used according to the standard ISO 22 196: (E) 2007. The results are summarised in the Table 3. Neat PVC matrix was used as the reference giving the Ut values. The test was performed for n-WF/PVC sample as well, and no antibacterial activity of unmodiﬁed WF was observed against either of the tested bacteria. Modiﬁcation of WF by either Ag or ZnO imparted moderate surface antibacterial activity R about 3 to the model composites towards both kinds of bacteria. Combination of Ag and ZnO in WF-Ag/ZnO resulted in enhanced activity R nearly about 5. WF-Ag/ZnO-AA was proved as the best performing m-WF among prepared ﬁllers. Excellent surface antibacterial activity was experienced testifying for total bactericidal effect against both used bacterial strains at used testing concentrations, so that no recovery of survival bacteria was observed. It means that the surface antibacterial performance of the material is fully comparable with the highest demanding requirements common in medical applications. We consider this result as a strong indication of the synergic effect between the two principally different antibacterial inorganic agents – nanosilver which is a metal and hierarchically nanostructured ZnO which is a semiconductor. Observed results are in agreement with previous studies reported from our laboratories (Bazant et al., 2014) and from others (Ghosh et al., 2012; Lu et al., 2008; Sadeghi, 2014). Besides that, the enhancement of antibacterial performance of prepared ﬁllers positively correlates with the increase of the complexity of ZnO hierarchical morphology which is in accordance with our other observations (Machovsky et al., 2014, In Press).
P. Bazant et al. / Industrial Crops and Products 62 (2014) 179–187
Table 3 Surface antibacterial activity evaluation of WF/PVC composites according ISO 22196: 2007 (E) (ISO, 2007). Sample code
Number of viable E. coli cells recovered per cm2 specimen, N (CFU/cm2 )
Number of viable S. aureus cells recovered per cm2 specimen, N (CFU/cm2 )
Antibacterial Activity a E. coli, R = Ut - At (Log CFU)
Antibacterial activity a S. aureus, R = Ut - At (Log CFU)
neat PVC WF/PVC WF-Ag/PVC WF-ZnO/PVC WF- Ag/ZnO/PVC WF-Ag-AA/PVC WF-ZnO-AA/PVC WF–Ag/ZnO-AA/PVC
6.9 × 106 9.5 × 106 7.5 × 103 7.3 × 103 2.4 × 102 1.3 × 103 3.6 × 104 <1
1.3 × 105 6.1 × 105 6.3 × 103 2.8 × 102 1.0 1.2 × 103 3.1 × 102 <1
Ut = 6.8 −0.14 2.9 3.0 4.5 3.7 2.3 >6.8
Ut = 5.1 -0.68 1.3 2.6 5.1 2.0 2.6 >5.1
a Each experiment was performed in triplicate and results passed more than sufﬁciently valid test criteria of the standard. Repeatability and reproducibility of the test are reported about 0.09 and 0.3 respectively in the standard. Therefore, the values of R are rounded to one decimal digit and the error can be estimated as several tenths.
4. Conclusions In a conclusion, nanosilver and nanostructured ZnO modiﬁed types of wood ﬂour were prepared by microwave assisted solvothermal synthesis and used as the active ﬁller for wood plastic composites imparting the surface antibacterial property to the material. The growth of inorganic particles decorating WF particles was described and the reaction mechanism was explained with respect to the used wood substrate components and chosen reaction conditions and synthesis protocol variation. Model m-WF/PVC composites were prepared in order to demonstrate the ﬁller functionality at only 5 %wt concentration. Moderate effect of single components (silver or ZnO modiﬁed WF) was observed, while combination in a hybrid Ag/ZnO material decorating the surface of WF particles showed enhanced performance. The synergy was more pronounced in case of material synthesised by the process facilitated with additional ammonia reaction step. These results proved that it is possible to obtain materials with excellent antimicrobial properties for potential hygienic or medical applications even for WPC. Acknowledgements The authors acknowledge the support of the Operational Programme ‘Education for Competitiveness’ co-funded by the European Social Fund (ESF) and the national budget of the Czech Republic, within the project ‘Advanced Theoretical and Experimental Studies of Polymer Systems’ (reg. number: CZ.1.07/2.3.00/20.0104). The authors also acknowledge the Operational Programme ‘Research and Development for Innovations’ co-funded by the European Regional Development Fund (ERDF) and the national budget of the Czech Republic, within the project ‘Centre of Polymer Systems’ (reg. number: CZ.1.05/2.1.00/03.0111). The work of L.M. and J.S. was also supported by the Internal Grant Agency of Tomas Bata University in Zlin; contract grant number: IGA/FT/2014/008. References  ISO 22196: 2007 (E) Plastics - Measurement of antibacterial activity on plastics surfaces. Geneva, Switzerland. Ashori, A., 2008. Wood-plastic composites as promising green-composites for automotive industries! Bioresource Technol. 99, 4661–4667. Bazant, P., Kuritka, I., Hudecek, O., Machovsky, M., Mrlik, M., Sedlacek, T., 2014. Microwave-assisted synthesis of Ag/ZnO hybrid ﬁller, preparation, and characterization of antibacterial poly(vinyl chloride) composites made from the same. Polym. Composite. 35, 19–26. Benthien, J.T., Thoemen, H., Maikowski, S., Lenz, M.T., 2012. Resistance of ﬂat-pressed wood-plastic composites to fungal decay: effects of wood ﬂour content, density, and manufacturing technology. Wood Fiber Sci. 44, 422–429. Biswick, T., Jones, W., Pacula, A., Serwicka, E., Podobinski, J., 2009. Evidence for the formation of anhydrous zinc acetate and acetic anhydride during the thermal
degradation of zinc hydroxy acetate, Zn5 (OH)8 (CH3 CO2 )2 ·4H2 O to ZnO. Solid State Sci. 11, 330–335. Chauhan, R., Kumar, A., Chaudhary, R.P., 2012. Photocatalytic studies of silver doped ZnO nanoparticles synthesized by chemical precipitation method. J. Sol-Gel Sci. Technol. 63, 546–553. Cho, S., Jung, S.H., Lee, K.H., 2008. Morphology-controlled growth of ZnO nanostructures using microwave irradiation: from basic to complex structures. J. Phys. Chem. C 112, 12769–12776. Dastjerdi, R., Montazer, M., 2010. A review on the application of inorganic nanostructured materials in the modiﬁcation of textiles: Focus on anti-microbial properties. Colloid. Surface. B 79, 5–18. Devi, R.R., Maji, T.K., 2008. Chemical modiﬁcation of rubber wood with styrene and glycidyl methacrylate. Polym. Composite. 29, 1258–1262. Droval, G., Aranberri, I., German, L., Ivanov, E., Dimitrova, E., Kotsilkova, R., Verelst, M., Dexpert-Ghys, J., 2014. Thermal and rheological characterization of antibacterial nanocomposites: poly(amide) 6 and low-density poly(ethylene) ﬁlled with zinc oxide. J. Thermoplast. Compos. Mater. 27, 268–284. Dwivedi, P., Narvi, S.S., Tewari, R.P., 2013. Application of polymer nanocomposites in the nanomedicine landscape: envisaging strategies to combat implant associated infections. J. Appl. Biomater. Funct. Mater. 11, 129–142. Fan, F.R., Ding, Y., Liu, D.Y., Tian, Z.Q., Wang, Z.L., 2009. Facet-selective epitaxial growth of heterogeneous nanostructures of semiconductor and metal: ZnO nanorods on Ag nanocrystals. J. Am. Chem. Soc. 131, 12036–12037. Farouk, A., Moussa, S., Ulbricht, M., Schollmeyer, E., Textor, T., 2014. ZnOmodiﬁed hybrid polymers as an antibacterial ﬁnish for textiles. Text. Res. J. 84, 40–51. Fowler, P.A., Hughes, J.M., Elias, R.M., 2006. Biocomposites: technology, environmental credentials and market forces. J. Sci. Food Agric. 86, 1781–1789. Ghosh, S., Goudar, V.S., Padmalekha, K.G., Bhat, S.V., Indi, S.S., Vasan, H.N., 2012. ZnO/Ag nanohybrid: synthesis, characterization, synergistic antibacterial activity and its mechanism. Rsc Adv. 2, 930–940. Golic, D.L., Brankovic, G., Vojisavljevic, K., Recnik, A., Daneu, N., Bernik, S., Scepanovic, M., Poleti, D., Brankovic, Z., 2011. Structural characterization of self-assembled ZnO nanoparticles obtained by the sol-gel method from Zn(CH3COO)2·2H2O. Nanotechnology 22, http://dx.doi.org/10.1088/0957-4484/22/39/395603, Art. No 395603 (9pp). Gowri, S., Almeida, L., Amorim, T., Carneiro, N., Souto, A.P., Esteves, M.F., 2010. Polymer nanocomposites for multifunctional ﬁnishing of textiles - a review. Text. Res. J. 80, 1290–1306. Guo, L.Y., Yuan, W.Y., Lu, Z.S., Li, C.M., 2013. Polymer/nanosilver composite coatings for antibacterial applications. Colloid. Surface. A 439, 69–83. Guzman, M., Dille, J., Godet, S., 2012. Synthesis and antibacterial activity of silver nanoparticles against gram-positive and gram-negative bacteria. Nanomedicine 8, 37–45. Hrabalova, M., Gregorova, A., Wimmer, R., Sedlarik, V., Machovsky, M., Mundigler, N., 2010. Effect of wood ﬂour loading and thermal annealing on viscoelastic properties of poly(lactic acid) composite ﬁlms. J. Appl. Polym. Sci. 118, 1534–1540. Huttermann, A., Mai, C., Kharazipour, A., 2001. Modiﬁcation of lignin for the production of new compounded materials. Appl. Microbiol. Biotechnol. 55, 387–394. Jayakumar, R., Prabaharan, M., Shalumon, K.T., Chennazhi, K.P., Nair, S.V., 2012. Biomedical Applications of Polymer/Silver Composite Nanoﬁbers. In: Jayakumar, R., Nair, S.V. (Eds.), Biomedical Applications of Polymeric Nanoﬁbers. SpringerVerlag, Berlin, pp. 263–282. Karas, M., Muszynski, L., 2011. Sustainable bio-composites for highway infrastructure: feasibility of material substitution in existing products. Bioresources 6, 3915–3932. Kartal, S.N., Aysal, S., Terzi, E., Yilgor, N., Yoshimura, T., Tsunoda, K., 2013. Wood and bamboo-PP composites: fungal and termite resistance, water absorption, and FT-IR analyses. Bioresources 8, 1222–1244. Li, X., Lei, B.R., Lin, Z.D., Huang, L.H., Tan, S.Z., Cai, X., 2013. The utilization of organic vermiculite to reinforce wood-plastic composites with higher ﬂexural and tensile properties. Ind. Crop. Prod. 51, 310–316. Lin, Z.Y., Renneckar, S., 2011. Nanocomposite-based lignocellulosic ﬁbers 2: layerby-layer modiﬁcation of wood ﬁbers for reinforcement in thermoplastic composites. Compos. Part A-Appl. Sci. 42, 84–91.
P. Bazant et al. / Industrial Crops and Products 62 (2014) 179–187 Llorens, A., Lloret, E., Picouet, P.A., Trbojevich, R., Fernandez, A., 2012. Metallic-based micro and nanocomposites in food contact materials and active food packaging. Trends Food Sci. Technol. 24, 19–29. Lopez-Naranjo, E.J., Alzate-Gaviria, L.M., Hernandez-Zarate, G., Reyes-Trujeque, J., Cupul-Manzano, C.V., Cruz-Estrada, R.H., 2013. Effect of biological degradation by termites on the ﬂexural properties of pinewood residue/recycled highdensity polyethylene composites. J. Appl. Polym. Sci. 128, 2595–2603. Lu, W.W., Liu, G.S., Gao, S.Y., Xing, S.T., Wang, J.J., 2008. Tyrosine-assisted preparation of Ag/ZnO nanocomposites with enhanced photocatalytic performance and synergistic antibacterial activities. Nanotechnology 19, Art. No 445711 (10pp). Machovsky, M., Kuritka, I., Bazant, P., Vesela, D., Saha, P., 2014. Antibacterial performance of ZnO-based ﬁllers with mesoscale structured morphology in model medical PVC composites. Mater. Sci. Eng. C, http://dx.doi.org/ 10.1016/j.msec.2014.04.034, In Press. Marambio-Jones, C., Hoek, E.M.V., 2010. A review of the antibacterial effects of silver nanomaterials and potential implications for human health and the environment. J. Nanopart. Res. 12, 1531–1551. Muller, M., Gellerich, A., Militz, H., Krause, A., 2013. Resistance of modiﬁed polyvinyl chloride/wood ﬂour composites to basidiomycetes. Eur J Wood Wood Prod 71, 199–204. Najaﬁ, S.K., 2013. Use of recycled plastics in wood plastic composites - a review. Waste Manage. 33, 1898–1905. Naumann, A., Stephan, I., Noll, M., 2012. Material resistance of weathered woodplastic composites against fungal decay. Int. Biodeter. Biodegr. 75, 28–35. Okamoto, T., 2003. Recent developments in wood/plastic composites - Extrusion of wood-based materials. Mokuzai Gakkaishi 49, 401–407. Richardson, J.J., Lange, F.F., 2009. Controlling Low Temperature Aqueous Synthesis of ZnO. 1. Thermodynamic Analysis. Cryst. Growth Design 9, 2570–2575. Sadeghi, B., 2014. Preparation of ZnO/Ag nanocomposite and coating on polymers for anti-infection biomaterial application. Spectrochim. Acta A 118, 787–792. Seil, J.T., Webster, T.J., 2011. Reduced Staphylococcus aureus proliferation and bioﬁlm formation on zinc oxide nanoparticle PVC composite surfaces. Acta Biomater. 7, 2579–2584.
Schauwecker, C., Morrell, J.J., McDonald, A.G., Fabiyi, J.S., 2006. Degradation of a wood-plastic composite exposed under tropical conditions. Forest Prod. J. 56, 123–129. Schilling, J.S., Norcutt, A., 2010. Effects of wood mixtures on deterioration by a ﬁlamentous brown-rot fungus. Wood Fiber Sci. 42, 150–157. Schirp, A., Ibach, R.E., Pendleton, D.E., Wolcott, M.P., 2008. Biological degradation of wood-plastic composites (WPC) and strategies for improving the resistance of WPC against biological decay. In: Development of Commercial Wood Preservatives: Efﬁcacy, Environmental, and Health Issues., pp. 480–507. Schwartz, V.B., Thetiot, F., Ritz, S., Putz, S., Choritz, L., Lappas, A., Forch, R., Landfester, K., Jonas, U., 2012. Antibacterial surface coatings from zinc oxide nanoparticles embedded in poly(N-isopropylacrylamide) hydrogel surface layers. Adv. Funct. Mater. 22, 2376–2386. Simonsen, J., Freitag, C.M., Silva, A., Morrell, J.J., 2004. Wood/plastic ratio: effect on performance of borate biocides against a brown rot fungus. Holzforschung 58, 205–208. Solpan, D., Guven, O., 1999. Preservation of beech and spruce wood by allyl alcoholbased copolymers. Radiat. Phys. Chem. 54, 583–591. Tascioglu, C., Yoshimura, T., Tsunoda, K., 2013. Biological performance of woodplastic composites containing zinc borate: laboratory and 3-year ﬁeld test results. Compos. Part B-Eng. 51, 185–190. Turku, I., Karki, T., 2014a. The effect of carbon ﬁbers, glass ﬁbers and nanoclay on wood ﬂour-polypropylene composite properties. Eur J Wood Wood Prod 72, 73–79. Turku, I., Karki, T., 2014b. Research progress in wood-plastic nanocomposites: a review. J. Thermoplast. Compos. Mater. 27, 180–204. Xu, K.M., Li, K.F., Yun, H., Zhong, T.H., Cao, X.L., 2013. A comparative study on the inhibitory ability of various wood-based composites against harmful biological species. Bioresources 8, 5749–5760. Zhang, Y., Gao, X.J., Zhi, L., Liu, X., Jiang, W., Sun, Y.H., Yang, J., 2014. The synergetic antibacterial activity of Ag islands on ZnO (Ag/ZnO) heterostructure nanoparticles and its mode of action. J. Inorg. Biochem. 130, 74–83. Zhao, M., Wu, D.P., Chang, J.L., Bai, Z.Y., Jiang, K., 2009. Synthesis of cup-like ZnO microcrystals via a CTAB-assisted hydrothermal route. Mater. Chem. Phys. 117, 422–424.